Microstructural evolution and phase HPT...Full length article Microstructural evolution and phase...
Embed Size (px)
Transcript of Microstructural evolution and phase HPT...Full length article Microstructural evolution and phase...
lable at ScienceDirect
Acta Materialia 109 (2016) 300e313
Contents lists avai
journal homepage: www.elsevier .com/locate/actamat
Full length article
Microstructural evolution and phase transformation in twinning-induced plasticity steel induced by high-pressure torsion
X.H. An a, *, Q.Y. Lin a, G. Sha b, M.X. Huang c, S.P. Ringer a, d, Y.T. Zhu b, e, X.Z. Liao a, **
a School of Aerospace, Mechanical and Mechatronic Engineering, The University of Sydney, Sydney, NSW 2006, Australiab School of Materials Science and Engineering, Nanjing University of Science and Technology, Jiangsu 210094, Chinac Department of Mechanical Engineering, The University of Hong Kong, Hong Kong, Chinad Australian Centre for Microscopy & Microanalysis, The University of Sydney, Sydney, NSW 2006, Australiae Department of Materials Science and Engineering, North Carolina State University, Raleigh, NC 27695, USA
a r t i c l e i n f o
Article history:Received 9 December 2015Received in revised form5 February 2016Accepted 19 February 2016Available online xxx
Keywords:Twinning-induced plasticity steelNanostructuresPhase transformationElement diffusion and segregationHigh-pressure torsion
* Corresponding author.** Corresponding author.
E-mail addresses: firstname.lastname@example.org (X.H. Anau (X.Z. Liao).
http://dx.doi.org/10.1016/j.actamat.2016.02.0451359-6454/ 2016 Acta Materialia Inc. Published by
a b s t r a c t
The microstructural evolution of twinning-induced plasticity steel during high-pressure torsion (HPT)processing at 573 K was systematically evaluated. Due to the high processing temperature, the formationof a homogeneous nanostructure was primarily dominated by complicated dislocation and grainboundary activities in lieu of deformation twinning. Apart from the grain refinement process, phasetransformation took place at late stages of deformation, resulting in the microstructural fingerprint ofequaxied nanograins with multiple phases in the steel. On account of remarkable elemental redistri-bution, the diffusion-controlled nature of the transformation was convincingly identified. During thetransformation, although the cementite also initially formed, austenite eventually decomposed intoferrite and Mn-riched M23C6 carbide, implying that Mn is the pivotal alloying element for the trans-formation kinetics. Owing to the sluggish bulk diffusivity of Mn, it is proposed that a high density ofdefects, nanostructures and the HPT processing play a crucial role in promoting the elemental diffusionand segregation and in stimulating the phase transformation.
2016 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.
Bulk ultrafine-grained (UFG, < 1000 nm) and nanocrystalline(NC, < 100 nm) materials have been extensively explored over thelast two decades due to their superior mechanical properties,including exceptionally high strength and hardness, excellent fa-tigue resistance and low-temperature superplasticity [1e5]. Severeplastic deformation (SPD) is among themost effective methods thatcan produce fully dense and contamination-free bulk UFG and NCmaterials [3e5]. By recourse to the SPD techniques, originallycoarse-grained structures can be substantially refined to UFG or NCstructures through a series of sophisticated grain refinement pro-cesses [3e5]. Comprehensive understanding of the fundamentalmechanisms of SPD-inducedmicrostructural evolution is crucial forachieving optimal mechanical properties of these materials viafine-tuning their microstructures.
It is well documented that dislocation activities and
Elsevier Ltd. All rights reserved.
deformation twinning are the two primary SPD-induced grainrefinement mechanisms . For materials in which dislocation slipis the dominant deformation mechanism, the SPD-induced micro-structural evolution is mainly controlled by complicated dislocationactivities that subdivide a large grain into many smaller volumeelements through the formation of dislocation cells. Withincreasing plastic strain, the cell boundaries gradually evolve intolow-angle and then high-angle grain boundaries (LAGBs andHAGBs, whose misorientation angles are below and above 15,respectively) [6,7]. In contrast, refinement via deformation twin-ning involves the formation of a high-density of nanoscale twins incoarse grains and the subsequent transformation of two-dimensional twin lamellae structures into three-dimensionalnanograins through extensive interactions between twin bound-aries (TBs) and other defects (mainly dislocations) . The finalgrain sizes after the refinement by the two mechanisms aregenerally in the range of submicrometer and nanometer, respec-tively [8,9]. In these bulk UFG and NC materials, there are aconsiderable fraction of LAGBs and a high density of dislocationsresided in or near non-equilibrium HAGBs, which remarkably in-fluence the thermal stability and mechanical properties of thematerials [10e12].
Delta:1_given nameDelta:1_surnameDelta:1_given nameDelta:1_surnameDelta:1_given nameDelta:1_surnameDelta:1_given namemailto:email@example.com:firstname.lastname@example.org:email@example.com://crossmark.crossref.org/dialog/?doi=10.1016/j.actamat.2016.02.045&domain=pdfwww.sciencedirect.com/science/journal/13596454www.elsevier.com/locate/actamathttp://dx.doi.org/10.1016/j.actamat.2016.02.045http://dx.doi.org/10.1016/j.actamat.2016.02.045http://dx.doi.org/10.1016/j.actamat.2016.02.045
X.H. An et al. / Acta Materialia 109 (2016) 300e313 301
In addition to grain refinement, SPD processing can also lead tothe formation of non-equilibrium solid solutions, disordering,amorphization, and phase transformations under high stress levelsin various alloys [13e16]. For example, SPD can dissolve cementitein pearlitic steels through extensive C-dislocation interactions ,promoting a reverse phase transformation from ferrite to austenite. Although the reverted austenitic phase is unstable at roomtemperature, the long-distance diffusion of C atoms, stemmed fromthe decomposition of cementite, stabilizes to some extent theaustenitic phase . Therefore, alloying elements dissolved in thematrix phase play a significant role in SPD-induced microstructuralevolution of engineering materials.
As a promising candidate for numerous industrial applications,twinning-induced plasticity (TWIP) steels with the austenitic phasehave been extensively investigated since they possess excellentcombination of high tensile strength and good ductility, whichoriginates from their exceptionally large work-hardening rate[17e20]. It is generally recognized that the high work-hardeningrate is closely related to the formation of deformation twins[19,20]. TBs act as effective barriers for dislocation motion tostrengthen the materials and the increasing density of TBs withfurther straining results in a dynamic Hall-Petch effect. Addi-tionally, the extensive interaction between the interstitial C atomsof CeMn dipoles and dislocations produces a dynamic strain agingeffects, also leading to high work-hardening rate . Based on thetraditional crystal plasticity theory, the activation of predominantdeformation mechanism is mainly controlled by the stacking faultenergy (SFE) , which is highly dependent on the chemicalcomposition of TWIP steels. Until now, most researches concerningTWIP steels focused on the dependence of deformation mecha-nisms on their alloying elements and SFE [23e26], and the prop-erties associated with microstructures [27e30]. Compared to otheradvanced steels [13,31e35], investigation on the microstructuralresponse of TWIP steels to SPD processing is still limited [37,38].However, fundamental exploration of the SPD-induced micro-structural evolution of TWIP steels is important both scientifically,for the comprehensive understanding of the grain refinementprocesses in the engineering metallic materials, and technologi-cally with respect to their energy absorption applications wherehigh strain will be imposed on the steels.
In present work, high-pressure torsion (HPT), which is one ofthe most popular SPD techniques , was applied to process aTWIP steel at 573 K. The HPT-induced microstructural evolutionwas systematically studied in virtue of various advanced charac-terization methods, including X-ray diffraction (XRD), conventionalelectron backscatter diffraction (EBSD), scanning electronmicroscope-transmission Kikuchi diffraction (SEM-TKD) andtransmission electron microscopy (TEM). During HPT processing,diffusional phase transformation surprisingly occurred via thedecomposition of austenite into ferrite and carbides. To link thephase transformation and elemental diffusion, atom probe to-mography (APT) was employed to analyze the elemental distribu-tions before and after HPT processing.
2. Experimental procedure
2.1. Materials and processing
The original TWIP steel used in this investigation is a commer-cial product produced by Ansteel Co. Ltd. in China. The nominalchemical composition of the TWIP steel is Fe-17.37Mn-3.31C-3.34Al-0.94Si in at.% or Fee18Mn-0.75C-1.7Al-0.5Si in wt.%.Detailed information about the material is available in Refs. [40,41].For HPT processing, the fully recrystallized steel was cut into discsamples with a diameter of 20 mm and a thickness of 1.5 mm. The
disks were HPT processed through 1, 5, 10, and 12 revolutions(thereafter referred to as 1R, 5R, 10R and 12R samples, respectively)under a quasi-constrained condition  with an imposed pressureof 4.0 GPa at 573 K. Before HPT processing, the anvils were pre-heated to 573 K and then held for 5 min to warm the samples.The temperature was kept at 573 10 K during the process. Thesamples were quenched into water immediately after HPT pro-ce